| Sample | Composition (mol%) | Composition (mol%) | Composition (mol%) | Composition (mol%) | Composition (mol%) | L (mm day-1) | Weathering durability | Appearance after putting in air for 150 days |
|        | P2O5               | PbBr2              | PbCl2              | PbO                | PbF2               |              |                       |                                              |
| 1      | 30                 | 20                 | 50                 |                    |                    | 7.9x10-5     | A                     | transparent, no visible change               |
| 2      | 30                 | 30                 | 40                 |                    |                    | 9x10-5       | A                     | transparent, no visible change               |
| 7      | 40                 |                    | 60                 |                    |                    | 1.0x10-4     | A                     | transparent, no visible change               |
| 8      | 40                 | 20                 | 40                 |                    |                    | 8.1x10-5     | B                     | translucent                                  |
| 9      | 40                 | 30                 | 30                 |                    |                    | 1.9x10-4     | B                     | translucent                                  |
| 10     | 50                 |                    | 50                 |                    |                    | 3.0x10-3     | C                     | translucent                                  |
| 11     | 50                 | 30                 | 20                 |                    |                    | 1.0x10-2     | D                     | powder, opaque                               |
| 12     | 60                 | 30                 | 10                 |                    |                    | 2.2x10-2     | D                     | powder, opaque                               |
| 13     | 70                 | 30                 |                    |                    |                    | 5.6x10-2     | D                     | powder, opaque                               |
| 3      | 28.5               | 28.5               | 38                 | 5                  |                    | 5x10-5       | A                     | transparent, no visible change               |
| 4      | 28.5               | 28.5               | 38                 |                    | 5                  | 9.8x10-5     | A                     | transparent, no visible change               |
| 5      | 28.5               | 28.5               | 38                 | 2.5                | 2.5                | 1.1x10-4     | A                     | transparent, no visible change               |

Caption: The weathering durability and dissolution rate of some glasses in PbBr2-PbCl2-PbF2-PbO-P2O5 systems a

You are provided with a table from a material science paper. Here are JSON templates for two types of numeric cells: "Other" and "Glass_Compound_Amount":
{"value": "xx", "type": "Other"}
{"value": "xx", "type": "Glass_Compound_Amount", "constituent": "xx", "unit": "xx", "material": "xx"}

Please describe all numeric cells in the above table following the JSON templates (proceeding by row in a left-right, top-down direction). For each cell, output one JSON description per line. For any unanswerable attributes in the templates, set their value to the placeholder "xx".

Cell Description:
{"value": "1", "type": "Other"}
{"value": "30", "type": "Glass_Compound_Amount", "constituent": "P2O5", "unit": "mol", "material": "1"}
{"value": "20", "type": "Glass_Compound_Amount", "constituent": "PbBr2", "unit": "mol", "material": "1"}
{"value": "50", "type": "Glass_Compound_Amount", "constituent": "PbCl2", "unit": "mol", "material": "1"}
{"value": "2", "type": "Other"}
{"value": "30", "type": "Glass_Compound_Amount", "constituent": "P2O5", "unit": "mol", "material": "2"}
{"value": "30", "type": "Glass_Compound_Amount", "constituent": "PbBr2", "unit": "mol", "material": "2"}
{"value": "40", "type": "Glass_Compound_Amount", "constituent": "PbCl2", "unit": "mol", "material": "2"}
{"value": "7", "type": "Other"}
{"value": "40", "type": "Glass_Compound_Amount", "constituent": "P2O5", "unit": "mol", "material": "7"}
{"value": "60", "type": "Glass_Compound_Amount", "constituent": "PbCl2", "unit": "mol", "material": "7"}
{"value": "8", "type": "Other"}
{"value": "40", "type": "Glass_Compound_Amount", "constituent": "P2O5", "unit": "mol", "material": "8"}
{"value": "20", "type": "Glass_Compound_Amount", "constituent": "PbBr2", "unit": "mol", "material": "8"}
{"value": "40", "type": "Glass_Compound_Amount", "constituent": "PbCl2", "unit": "mol", "material": "8"}
{"value": "9", "type": "Other"}
{"value": "40", "type": "Glass_Compound_Amount", "constituent": "P2O5", "unit": "mol", "material": "9"}
{"value": "30", "type": "Glass_Compound_Amount", "constituent": "PbBr2", "unit": "mol", "material": "9"}
{"value": "30", "type": "Glass_Compound_Amount", "constituent": "PbCl2", "unit": "mol", "material": "9"}
{"value": "10", "type": "Other"}
{"value": "50", "type": "Glass_Compound_Amount", "constituent": "P2O5", "unit": "mol", "material": "10"}
{"value": "50", "type": "Glass_Compound_Amount", "constituent": "PbCl2", "unit": "mol", "material": "10"}
{"value": "11", "type": "Other"}
{"value": "50", "type": "Glass_Compound_Amount", "constituent": "P2O5", "unit": "mol", "material": "11"}
{"value": "30", "type": "Glass_Compound_Amount", "constituent": "PbBr2", "unit": "mol", "material": "11"}
{"value": "20", "type": "Glass_Compound_Amount", "constituent": "PbCl2", "unit": "mol", "material": "11"}
{"value": "12", "type": "Other"}
{"value": "60", "type": "Glass_Compound_Amount", "constituent": "P2O5", "unit": "mol", "material": "12"}
{"value": "30", "type": "Glass_Compound_Amount", "constituent": "PbBr2", "unit": "mol", "material": "12"}
{"value": "10", "type": "Glass_Compound_Amount", "constituent": "PbCl2", "unit": "mol", "material": "12"}
{"value": "13", "type": "Other"}
{"value": "70", "type": "Glass_Compound_Amount", "constituent": "P2O5", "unit": "mol", "material": "13"}
{"value": "30", "type": "Glass_Compound_Amount", "constituent": "PbBr2", "unit": "mol", "material": "13"}
{"value": "3", "type": "Other"}
{"value": "28.5", "type": "Glass_Compound_Amount", "constituent": "P2O5", "unit": "mol", "material": "3"}
{"value": "28.5", "type": "Glass_Compound_Amount", "constituent": "PbBr2", "unit": "mol", "material": "3"}
{"value": "38", "type": "Glass_Compound_Amount", "constituent": "PbCl2", "unit": "mol", "material": "3"}
{"value": "5", "type": "Glass_Compound_Amount", "constituent": "PbO", "unit": "mol", "material": "3"}
{"value": "4", "type": "Other"}
{"value": "28.5", "type": "Glass_Compound_Amount", "constituent": "P2O5", "unit": "mol", "material": "4"}
{"value": "28.5", "type": "Glass_Compound_Amount", "constituent": "PbBr2", "unit": "mol", "material": "4"}
{"value": "38", "type": "Glass_Compound_Amount", "constituent": "PbCl2", "unit": "mol", "material": "4"}
{"value": "5", "type": "Glass_Compound_Amount", "constituent": "PbF2", "unit": "mol", "material": "4"}
{"value": "5", "type": "Other"}
{"value": "28.5", "type": "Glass_Compound_Amount", "constituent": "P2O5", "unit": "mol", "material": "5"}
{"value": "28.5", "type": "Glass_Compound_Amount", "constituent": "PbBr2", "unit": "mol", "material": "5"}
{"value": "38", "type": "Glass_Compound_Amount", "constituent": "PbCl2", "unit": "mol", "material": "5"}
{"value": "2.5", "type": "Glass_Compound_Amount", "constituent": "PbO", "unit": "mol", "material": "5"}
{"value": "2.5", "type": "Glass_Compound_Amount", "constituent": "PbF2", "unit": "mol", "material": "5"}